#------------------------------------------------------------------------------
#$Date: 2021-05-22 10:32:51 +0300 (Sat, 22 May 2021) $
#$Revision: 265457 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/28/1562830.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1562830
loop_
_publ_author_name
'Kangas, Michael J.'
'Treadwell, LaRico J.'
'Haldolaarachchige, Neel'
'McAlpin, Jacob D.'
'Young, David P.'
'Chan, Julia Y.'
_publ_section_title
;
 Magnetic and electrical properties of flux grown single crystals of
 Ln6M4Al43 (Ln=Gd, Yb; M=Cr, Mo, W)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              523
_journal_page_last               531
_journal_paper_doi               10.1016/j.jssc.2012.08.022
_journal_volume                  197
_journal_year                    2013
_chemical_formula_moiety         'Al42.85 Gd6 Mo4.15'
_chemical_formula_sum            'Al42.85 Gd6 Mo4.15'
_chemical_formula_weight         2497.74
_space_group_IT_number           193
_space_group_name_Hall           '-P 6c 2'
_space_group_name_H-M_alt        'P 63/m c m'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2'
_symmetry_space_group_name_H-M   'P 63/m c m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   11.0189(10)
_cell_length_b                   11.0189(10)
_cell_length_c                   17.7799(15)
_cell_measurement_reflns_used    3972
_cell_measurement_temperature    293(1)
_cell_measurement_theta_max      30.999
_cell_measurement_theta_min      0.998
_cell_volume                     1869.5(3)
_computing_cell_refinement       'Denzo and Scalepack(Otwinski & Minor 1999)'
_computing_data_collection       'COLLECT (Nonius 1999)'
_computing_data_reduction        'Denzo and Scalepack(Otwinski & Minor 1999)'
_computing_molecular_graphics    'Crystal Maker'
_computing_publication_material  Publcif
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SIR 97'
_diffrn_ambient_temperature      293(1)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Nonius Kappa CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0296
_diffrn_reflns_av_sigmaI/netI    0.0161
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            7378
_diffrn_reflns_theta_full        30.97
_diffrn_reflns_theta_max         30.97
_diffrn_reflns_theta_min         2.13
_exptl_absorpt_coefficient_mu    12.844
_exptl_absorpt_correction_T_max  0.5660
_exptl_absorpt_correction_T_min  0.5660
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'HKL Scalepack'
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    4.437
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       fragment
_exptl_crystal_F_000             2231
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.198
_refine_diff_density_min         -1.137
_refine_diff_density_rms         0.153
_refine_ls_extinction_coef       0.00081(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.114
_refine_ls_matrix_type           full
_refine_ls_number_parameters     54
_refine_ls_number_reflns         1104
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.114
_refine_ls_R_factor_all          0.0190
_refine_ls_R_factor_gt           0.0176
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0131P)²+8.6740P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0398
_refine_ls_wR_factor_ref         0.0403
_reflns_number_gt                1050
_reflns_number_total             1104
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            JSSC-2013-197-523.cif
_cod_data_source_block           Gd6Mo4Al43
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Hexagonal' was changed to
'hexagonal' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_Hall     '-P 6c 2 '
_cod_database_code               1562830
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-y, x-y, z'
'-x+y, -x, z'
'x-y, x, z+1/2'
'y, -x+y, z+1/2'
'x-y, -y, -z+1/2'
'-x, -x+y, -z+1/2'
'y, x, -z+1/2'
'-y, -x, -z'
'x, x-y, -z'
'-x+y, y, -z'
'-x, -y, -z'
'x, y, -z-1/2'
'y, -x+y, -z'
'x-y, x, -z'
'-x+y, -x, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, y, z-1/2'
'x, x-y, z-1/2'
'-y, -x, z-1/2'
'y, x, z'
'-x, -x+y, z'
'x-y, -y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Gd1 Gd 0.469694(17) 0.0000 0.095044(11) 0.00917(7) Uani 1 2 d S . .
Mo1 Mo 0.26856(4) 0.0000 0.2500 0.00545(10) Uani 1 4 d S . .
Mo2 Mo 0.0000 0.0000 0.0000 0.00571(14) Uani 1 12 d S . .
Al1 Al 0.23573(9) 0.39396(9) 0.16413(5) 0.01010(17) Uani 1 1 d . . .
Al2 Al 0.15959(11) 0.0000 0.11451(7) 0.0099(2) Uani 1 2 d S . .
Al3 Al 0.25364(11) 0.0000 0.53028(7) 0.0095(2) Uani 1 2 d S . .
Al4 Al 0.14687(13) 0.55042(12) 0.2500 0.0099(2) Uani 1 2 d S . .
Al5 Al 0.24706(6) 0.49413(13) 0.0000 0.0113(2) Uani 1 2 d S . .
Al6 Al 0.3333 0.6667 0.12699(8) 0.0096(4) Uani 0.959(3) 3 d SP . .
Mo3 Mo 0.3333 0.6667 0.12699(8) 0.0096(4) Uani 0.041(3) 3 d SP . .
Al7 Al 0.85233(16) 0.0000 0.2500 0.0091(3) Uani 1 4 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Al1 Gd1 Al1 58.92(3) 23_655 3_655
Al1 Gd1 Al4 53.16(3) 23_655 9
Al1 Gd1 Al4 81.16(3) 3_655 9
Al1 Gd1 Al4 81.16(3) 23_655 4
Al1 Gd1 Al4 53.16(3) 3_655 4
Al4 Gd1 Al4 53.90(4) 9 4
Al1 Gd1 Al5 96.69(3) 23_655 15
Al1 Gd1 Al5 149.85(3) 3_655 15
Al4 Gd1 Al5 98.64(2) 9 15
Al4 Gd1 Al5 147.11(2) 4 15
Al1 Gd1 Al5 149.85(3) 23_655 4
Al1 Gd1 Al5 96.69(3) 3_655 4
Al4 Gd1 Al5 147.11(2) 9 4
Al4 Gd1 Al5 98.64(2) 4 4
Al5 Gd1 Al5 99.05(3) 15 4
Al1 Gd1 Mo3 50.872(19) 23_655 22
Al1 Gd1 Mo3 109.40(2) 3_655 22
Al4 Gd1 Mo3 52.96(3) 9 22
Al4 Gd1 Mo3 106.58(3) 4 22
Al5 Gd1 Mo3 52.17(3) 15 22
Al5 Gd1 Mo3 151.21(3) 4 22
Al1 Gd1 Al6 50.872(19) 23_655 22
Al1 Gd1 Al6 109.40(2) 3_655 22
Al4 Gd1 Al6 52.96(3) 9 22
Al4 Gd1 Al6 106.58(3) 4 22
Al5 Gd1 Al6 52.17(3) 15 22
Al5 Gd1 Al6 151.21(3) 4 22
Mo3 Gd1 Al6 0.00(5) 22 22
Al1 Gd1 Mo3 109.40(2) 23_655 1_545
Al1 Gd1 Mo3 50.872(19) 3_655 1_545
Al4 Gd1 Mo3 106.58(3) 9 1_545
Al4 Gd1 Mo3 52.96(3) 4 1_545
Al5 Gd1 Mo3 151.21(3) 15 1_545
Al5 Gd1 Mo3 52.17(3) 4 1_545
Mo3 Gd1 Mo3 156.59(4) 22 1_545
Al6 Gd1 Mo3 156.59(4) 22 1_545
Al1 Gd1 Al6 109.40(2) 23_655 1_545
Al1 Gd1 Al6 50.872(19) 3_655 1_545
Al4 Gd1 Al6 106.58(3) 9 1_545
Al4 Gd1 Al6 52.96(3) 4 1_545
Al5 Gd1 Al6 151.21(3) 15 1_545
Al5 Gd1 Al6 52.17(3) 4 1_545
Mo3 Gd1 Al6 156.59(4) 22 1_545
Al6 Gd1 Al6 156.59(4) 22 1_545
Mo3 Gd1 Al6 0.00(5) 1_545 1_545
Al1 Gd1 Al3 54.41(2) 23_655 2_654
Al1 Gd1 Al3 54.41(2) 3_655 2_654
Al4 Gd1 Al3 106.89(3) 9 2_654
Al4 Gd1 Al3 106.89(3) 4 2_654
Al5 Gd1 Al3 97.87(2) 15 2_654
Al5 Gd1 Al3 97.87(2) 4 2_654
Mo3 Gd1 Al3 88.030(10) 22 2_654
Al6 Gd1 Al3 88.030(10) 22 2_654
Mo3 Gd1 Al3 88.030(10) 1_545 2_654
Al6 Gd1 Al3 88.030(10) 1_545 2_654
Al1 Gd1 Al3 146.93(2) 23_655 14_556
Al1 Gd1 Al3 146.93(2) 3_655 14_556
Al4 Gd1 Al3 128.89(3) 9 14_556
Al4 Gd1 Al3 128.89(3) 4 14_556
Al5 Gd1 Al3 50.97(2) 15 14_556
Al5 Gd1 Al3 50.97(2) 4 14_556
Mo3 Gd1 Al3 101.219(16) 22 14_556
Al6 Gd1 Al3 101.219(16) 22 14_556
Mo3 Gd1 Al3 101.218(16) 1_545 14_556
Al6 Gd1 Al3 101.218(16) 1_545 14_556
Al3 Gd1 Al3 116.20(2) 2_654 14_556
Al7 Mo1 Al7 66.59(8) 3_545 4_665
Al7 Mo1 Al4 178.10(5) 3_545 9
Al7 Mo1 Al4 115.31(5) 4_665 9
Al7 Mo1 Al4 115.31(5) 3_545 4
Al7 Mo1 Al4 178.10(5) 4_665 4
Al4 Mo1 Al4 62.79(6) 9 4
Al7 Mo1 Al2 68.11(3) 3_545 .
Al7 Mo1 Al2 68.11(3) 4_665 .
Al4 Mo1 Al2 112.38(2) 9 .
Al4 Mo1 Al2 112.38(2) 4 .
Al7 Mo1 Al2 68.11(3) 3_545 14_556
Al7 Mo1 Al2 68.11(3) 4_665 14_556
Al4 Mo1 Al2 112.38(2) 9 14_556
Al4 Mo1 Al2 112.38(2) 4 14_556
Al2 Mo1 Al2 127.01(6) . 14_556
Al7 Mo1 Al1 118.65(4) 3_545 9
Al7 Mo1 Al1 64.63(4) 4_665 9
Al4 Mo1 Al1 62.82(3) 9 9
Al4 Mo1 Al1 113.88(3) 4 9
Al2 Mo1 Al1 121.06(2) . 9
Al2 Mo1 Al1 60.74(2) 14_556 9
Al7 Mo1 Al1 64.63(4) 3_545 4
Al7 Mo1 Al1 118.65(4) 4_665 4
Al4 Mo1 Al1 113.88(3) 9 4
Al4 Mo1 Al1 62.82(3) 4 4
Al2 Mo1 Al1 60.74(2) . 4
Al2 Mo1 Al1 121.06(2) 14_556 4
Al1 Mo1 Al1 176.50(4) 9 4
Al7 Mo1 Al1 64.63(4) 3_545 17_556
Al7 Mo1 Al1 118.65(4) 4_665 17_556
Al4 Mo1 Al1 113.88(3) 9 17_556
Al4 Mo1 Al1 62.82(3) 4 17_556
Al2 Mo1 Al1 121.06(2) . 17_556
Al2 Mo1 Al1 60.74(2) 14_556 17_556
Al1 Mo1 Al1 111.59(4) 9 17_556
Al1 Mo1 Al1 68.29(4) 4 17_556
Al7 Mo1 Al1 118.65(4) 3_545 22
Al7 Mo1 Al1 64.63(4) 4_665 22
Al4 Mo1 Al1 62.82(3) 9 22
Al4 Mo1 Al1 113.88(3) 4 22
Al2 Mo1 Al1 60.74(2) . 22
Al2 Mo1 Al1 121.06(2) 14_556 22
Al1 Mo1 Al1 68.29(4) 9 22
Al1 Mo1 Al1 111.59(4) 4 22
Al1 Mo1 Al1 176.50(4) 17_556 22
Al7 Mo1 Gd1 121.595(16) 3_545 14_556
Al7 Mo1 Gd1 121.595(16) 4_665 14_556
Al4 Mo1 Gd1 57.653(13) 9 14_556
Al4 Mo1 Gd1 57.653(13) 4 14_556
Al2 Mo1 Gd1 167.68(3) . 14_556
Al2 Mo1 Gd1 65.31(3) 14_556 14_556
Al1 Mo1 Gd1 62.84(2) 9 14_556
Al1 Mo1 Gd1 114.72(2) 4 14_556
Al1 Mo1 Gd1 62.84(2) 17_556 14_556
Al1 Mo1 Gd1 114.72(2) 22 14_556
Al7 Mo1 Gd1 121.595(16) 3_545 .
Al7 Mo1 Gd1 121.595(16) 4_665 .
Al4 Mo1 Gd1 57.653(13) 9 .
Al4 Mo1 Gd1 57.653(13) 4 .
Al2 Mo1 Gd1 65.31(3) . .
Al2 Mo1 Gd1 167.68(3) 14_556 .
Al1 Mo1 Gd1 114.72(2) 9 .
Al1 Mo1 Gd1 62.84(2) 4 .
Al1 Mo1 Gd1 114.72(2) 17_556 .
Al1 Mo1 Gd1 62.84(2) 22 .
Gd1 Mo1 Gd1 102.372(15) 14_556 .
Al2 Mo2 Al2 180.00(3) 15 3
Al2 Mo2 Al2 68.96(4) 15 13
Al2 Mo2 Al2 111.04(4) 3 13
Al2 Mo2 Al2 111.04(4) 15 .
Al2 Mo2 Al2 68.96(4) 3 .
Al2 Mo2 Al2 180.00(3) 13 .
Al2 Mo2 Al2 68.96(4) 15 16
Al2 Mo2 Al2 111.04(4) 3 16
Al2 Mo2 Al2 68.96(4) 13 16
Al2 Mo2 Al2 111.04(4) . 16
Al2 Mo2 Al2 111.04(4) 15 4
Al2 Mo2 Al2 68.96(4) 3 4
Al2 Mo2 Al2 111.04(4) 13 4
Al2 Mo2 Al2 68.96(4) . 4
Al2 Mo2 Al2 180.00(10) 16 4
Al2 Mo2 Al3 62.35(2) 15 17_556
Al2 Mo2 Al3 117.65(2) 3 17_556
Al2 Mo2 Al3 62.35(2) 13 17_556
Al2 Mo2 Al3 117.65(2) . 17_556
Al2 Mo2 Al3 119.92(4) 16 17_556
Al2 Mo2 Al3 60.08(4) 4 17_556
Al2 Mo2 Al3 117.65(2) 15 5_554
Al2 Mo2 Al3 62.35(2) 3 5_554
Al2 Mo2 Al3 117.65(2) 13 5_554
Al2 Mo2 Al3 62.35(2) . 5_554
Al2 Mo2 Al3 60.08(4) 16 5_554
Al2 Mo2 Al3 119.92(4) 4 5_554
Al3 Mo2 Al3 180.00(10) 17_556 5_554
Al2 Mo2 Al3 119.92(4) 15 18_556
Al2 Mo2 Al3 60.08(4) 3 18_556
Al2 Mo2 Al3 62.35(2) 13 18_556
Al2 Mo2 Al3 117.65(2) . 18_556
Al2 Mo2 Al3 62.35(2) 16 18_556
Al2 Mo2 Al3 117.65(2) 4 18_556
Al3 Mo2 Al3 116.509(16) 17_556 18_556
Al3 Mo2 Al3 63.491(16) 5_554 18_556
Al2 Mo2 Al3 62.35(2) 15 14_556
Al2 Mo2 Al3 117.65(2) 3 14_556
Al2 Mo2 Al3 119.92(4) 13 14_556
Al2 Mo2 Al3 60.08(4) . 14_556
Al2 Mo2 Al3 62.35(2) 16 14_556
Al2 Mo2 Al3 117.65(2) 4 14_556
Al3 Mo2 Al3 116.509(16) 17_556 14_556
Al3 Mo2 Al3 63.491(16) 5_554 14_556
Al3 Mo2 Al3 116.509(16) 18_556 14_556
Al2 Mo2 Al3 117.65(2) 15 2_554
Al2 Mo2 Al3 62.35(2) 3 2_554
Al2 Mo2 Al3 60.08(4) 13 2_554
Al2 Mo2 Al3 119.92(4) . 2_554
Al2 Mo2 Al3 117.65(2) 16 2_554
Al2 Mo2 Al3 62.35(2) 4 2_554
Al3 Mo2 Al3 63.491(16) 17_556 2_554
Al3 Mo2 Al3 116.509(16) 5_554 2_554
Al3 Mo2 Al3 63.491(16) 18_556 2_554
Al3 Mo2 Al3 180.00(5) 14_556 2_554
Al2 Mo2 Al3 60.08(4) 15 6_554
Al2 Mo2 Al3 119.92(4) 3 6_554
Al2 Mo2 Al3 117.65(2) 13 6_554
Al2 Mo2 Al3 62.35(2) . 6_554
Al2 Mo2 Al3 117.65(2) 16 6_554
Al2 Mo2 Al3 62.35(2) 4 6_554
Al3 Mo2 Al3 63.491(16) 17_556 6_554
Al3 Mo2 Al3 116.509(16) 5_554 6_554
Al3 Mo2 Al3 180.00(5) 18_556 6_554
Al3 Mo2 Al3 63.491(16) 14_556 6_554
Al3 Mo2 Al3 116.509(16) 2_554 6_554
Al6 Al1 Mo1 116.57(4) . 3
Al6 Al1 Al2 128.98(5) . 3
Mo1 Al1 Al2 59.12(3) 3 3
Al6 Al1 Al4 62.25(4) . 3_665
Mo1 Al1 Al4 108.23(3) 3 3_665
Al2 Al1 Al4 165.04(5) 3 3_665
Al6 Al1 Al4 61.45(3) . .
Mo1 Al1 Al4 58.08(3) 3 .
Al2 Al1 Al4 107.20(4) 3 .
Al4 Al1 Al4 67.85(5) 3_665 .
Al6 Al1 Al7 161.40(5) . 4_665
Mo1 Al1 Al7 55.07(2) 3 4_665
Al2 Al1 Al7 63.91(4) 3 4_665
Al4 Al1 Al7 102.82(4) 3_665 4_665
Al4 Al1 Al7 103.71(3) . 4_665
Al6 Al1 Al3 107.18(5) . 5_554
Mo1 Al1 Al3 119.50(4) 3 5_554
Al2 Al1 Al3 61.14(4) 3 5_554
Al4 Al1 Al3 128.89(4) 3_665 5_554
Al4 Al1 Al3 155.23(4) . 5_554
Al7 Al1 Al3 90.78(3) 4_665 5_554
Al6 Al1 Gd1 67.96(2) . 4_665
Mo1 Al1 Gd1 168.71(4) 3 4_665
Al2 Al1 Gd1 127.25(4) 3 4_665
Al4 Al1 Gd1 63.83(3) 3_665 4_665
Al4 Al1 Gd1 121.52(4) . 4_665
Al7 Al1 Gd1 117.19(3) 4_665 4_665
Al3 Al1 Gd1 66.12(3) 5_554 4_665
Al6 Al1 Gd1 63.96(2) . 3
Mo1 Al1 Gd1 70.63(2) 3 3
Al2 Al1 Gd1 68.08(3) 3 3
Al4 Al1 Gd1 117.31(4) 3_665 3
Al4 Al1 Gd1 59.62(2) . 3
Al7 Al1 Gd1 120.16(4) 4_665 3
Al3 Al1 Gd1 95.76(3) 5_554 3
Gd1 Al1 Gd1 119.70(3) 4_665 3
Mo2 Al2 Mo1 165.67(5) . .
Mo2 Al2 Al1 123.42(3) . 22
Mo1 Al2 Al1 60.14(3) . 22
Mo2 Al2 Al1 123.42(3) . 4
Mo1 Al2 Al1 60.14(3) . 4
Al1 Al2 Al1 110.60(5) 22 4
Mo2 Al2 Al3 62.75(4) . 14_556
Mo1 Al2 Al3 131.58(6) . 14_556
Al1 Al2 Al3 97.12(4) 22 14_556
Al1 Al2 Al3 97.12(4) 4 14_556
Mo2 Al2 Al3 61.49(3) . 6_554
Mo1 Al2 Al3 121.56(3) . 6_554
Al1 Al2 Al3 157.06(6) 22 6_554
Al1 Al2 Al3 62.21(3) 4 6_554
Al3 Al2 Al3 64.07(3) 14_556 6_554
Mo2 Al2 Al3 61.49(3) . 5_554
Mo1 Al2 Al3 121.56(3) . 5_554
Al1 Al2 Al3 62.21(3) 22 5_554
Al1 Al2 Al3 157.06(6) 4 5_554
Al3 Al2 Al3 64.07(3) 14_556 5_554
Al3 Al2 Al3 115.05(6) 6_554 5_554
Mo2 Al2 Al7 114.15(4) . 4_665
Mo1 Al2 Al7 53.94(2) . 4_665
Al1 Al2 Al7 59.58(4) 22 4_665
Al1 Al2 Al7 106.26(4) 4 4_665
Al3 Al2 Al7 151.43(3) 14_556 4_665
Al3 Al2 Al7 142.17(5) 6_554 4_665
Al3 Al2 Al7 89.02(3) 5_554 4_665
Mo2 Al2 Al7 114.15(4) . 3_545
Mo1 Al2 Al7 53.94(2) . 3_545
Al1 Al2 Al7 106.26(4) 22 3_545
Al1 Al2 Al7 59.58(4) 4 3_545
Al3 Al2 Al7 151.43(3) 14_556 3_545
Al3 Al2 Al7 89.02(3) 6_554 3_545
Al3 Al2 Al7 142.17(5) 5_554 3_545
Al7 Al2 Al7 57.14(6) 4_665 3_545
Mo2 Al2 Gd1 125.04(4) . .
Mo1 Al2 Gd1 69.29(3) . .
Al1 Al2 Gd1 64.26(3) 22 .
Al1 Al2 Gd1 64.26(3) 4 .
Al3 Al2 Gd1 62.29(4) 14_556 .
Al3 Al2 Gd1 94.17(3) 6_554 .
Al3 Al2 Gd1 94.17(3) 5_554 .
Al7 Al2 Gd1 113.67(4) 4_665 .
Al7 Al2 Gd1 113.67(4) 3_545 .
Al5 Al3 Al5 118.72(5) 6 17_556
Al5 Al3 Al2 89.62(3) 6 14_556
Al5 Al3 Al2 89.62(3) 17_556 14_556
Al5 Al3 Mo2 115.13(3) 6 2
Al5 Al3 Mo2 115.13(3) 17_556 2
Al2 Al3 Mo2 57.17(3) 14_556 2
Al5 Al3 Al2 87.70(3) 6 5
Al5 Al3 Al2 150.84(5) 17_556 5
Al2 Al3 Al2 103.59(5) 14_556 5
Mo2 Al3 Al2 56.16(3) 2 5
Al5 Al3 Al2 150.84(5) 6 6
Al5 Al3 Al2 87.70(3) 17_556 6
Al2 Al3 Al2 103.59(5) 14_556 6
Mo2 Al3 Al2 56.16(3) 2 6
Al2 Al3 Al2 64.12(6) 5 6
Al5 Al3 Al1 66.65(2) 6 6
Al5 Al3 Al1 120.01(5) 17_556 6
Al2 Al3 Al1 148.07(2) 14_556 6
Mo2 Al3 Al1 112.57(4) 2 6
Al2 Al3 Al1 56.64(3) 5 6
Al2 Al3 Al1 90.19(5) 6 6
Al5 Al3 Al1 120.01(5) 6 20_556
Al5 Al3 Al1 66.65(2) 17_556 20_556
Al2 Al3 Al1 148.07(2) 14_556 20_556
Mo2 Al3 Al1 112.57(4) 2 20_556
Al2 Al3 Al1 90.19(5) 5 20_556
Al2 Al3 Al1 56.64(3) 6 20_556
Al1 Al3 Al1 62.80(4) 6 20_556
Al5 Al3 Al3 147.58(7) 6 15_556
Al5 Al3 Al3 56.87(3) 17_556 15_556
Al2 Al3 Al3 59.49(4) 14_556 15_556
Mo2 Al3 Al3 58.255(8) 2 15_556
Al2 Al3 Al3 107.76(4) 5 15_556
Al2 Al3 Al3 56.44(3) 6 15_556
Al1 Al3 Al3 145.57(6) 6 15_556
Al1 Al3 Al3 89.01(4) 20_556 15_556
Al5 Al3 Al3 56.87(3) 6 16_556
Al5 Al3 Al3 147.58(7) 17_556 16_556
Al2 Al3 Al3 59.49(4) 14_556 16_556
Mo2 Al3 Al3 58.255(8) 2 16_556
Al2 Al3 Al3 56.44(3) 5 16_556
Al2 Al3 Al3 107.76(4) 6 16_556
Al1 Al3 Al3 89.01(4) 6 16_556
Al1 Al3 Al3 145.57(6) 20_556 16_556
Al3 Al3 Al3 107.83(5) 15_556 16_556
Al5 Al3 Gd1 68.25(3) 6 2_655
Al5 Al3 Gd1 68.25(3) 17_556 2_655
Al2 Al3 Gd1 132.62(5) 14_556 2_655
Mo2 Al3 Gd1 170.21(5) 2 2_655
Al2 Al3 Gd1 116.11(4) 5 2_655
Al2 Al3 Gd1 116.11(4) 6 2_655
Al1 Al3 Gd1 59.48(3) 6 2_655
Al1 Al3 Gd1 59.48(3) 20_556 2_655
Al3 Al3 Gd1 124.298(5) 15_556 2_655
Al3 Al3 Gd1 124.298(5) 16_556 2_655
Al5 Al3 Gd1 61.47(2) 6 14_556
Al5 Al3 Gd1 61.47(2) 17_556 14_556
Al2 Al3 Gd1 68.82(4) 14_556 14_556
Mo2 Al3 Gd1 125.99(4) 2 14_556
Al2 Al3 Gd1 147.58(3) 5 14_556
Al2 Al3 Gd1 147.58(3) 6 14_556
Al1 Al3 Gd1 113.03(4) 6 14_556
Al1 Al3 Gd1 113.03(4) 20_556 14_556
Al3 Al3 Gd1 95.45(4) 15_556 14_556
Al3 Al3 Gd1 95.45(4) 16_556 14_556
Gd1 Al3 Gd1 63.80(2) 2_655 14_556
Mo1 Al4 Al1 136.93(4) 3 17_566
Mo1 Al4 Al1 136.93(4) 3 4_565
Al1 Al4 Al1 67.24(5) 17_566 4_565
Mo1 Al4 Al4 58.61(3) 3 8
Al1 Al4 Al4 92.25(3) 17_566 8
Al1 Al4 Al4 92.25(3) 4_565 8
Mo1 Al4 Al1 59.10(3) 3 14_556
Al1 Al4 Al1 109.97(4) 17_566 14_556
Al1 Al4 Al1 160.22(6) 4_565 14_556
Al4 Al4 Al1 107.50(3) 8 14_556
Mo1 Al4 Al1 59.10(3) 3 .
Al1 Al4 Al1 160.22(6) 17_566 .
Al1 Al4 Al1 109.97(4) 4_565 .
Al4 Al4 Al1 107.50(3) 8 .
Al1 Al4 Al1 65.57(5) 14_556 .
Mo1 Al4 Mo3 113.82(3) 3 14_556
Al1 Al4 Mo3 58.20(2) 17_566 14_556
Al1 Al4 Mo3 109.18(4) 4_565 14_556
Al4 Al4 Mo3 128.94(3) 8 14_556
Al1 Al4 Mo3 57.52(2) 14_556 14_556
Al1 Al4 Mo3 107.43(5) . 14_556
Mo1 Al4 Al6 113.82(3) 3 14_556
Al1 Al4 Al6 58.20(2) 17_566 14_556
Al1 Al4 Al6 109.18(4) 4_565 14_556
Al4 Al4 Al6 128.94(3) 8 14_556
Al1 Al4 Al6 57.52(2) 14_556 14_556
Al1 Al4 Al6 107.43(5) . 14_556
Mo3 Al4 Al6 0.00(4) 14_556 14_556
Mo1 Al4 Al6 113.82(3) 3 .
Al1 Al4 Al6 109.18(4) 17_566 .
Al1 Al4 Al6 58.20(2) 4_565 .
Al4 Al4 Al6 128.94(3) 8 .
Al1 Al4 Al6 107.43(5) 14_556 .
Al1 Al4 Al6 57.52(2) . .
Mo3 Al4 Al6 101.17(5) 14_556 .
Al6 Al4 Al6 101.17(5) 14_556 .
Mo1 Al4 Gd1 75.03(2) 3 3
Al1 Al4 Gd1 122.19(4) 17_566 3
Al1 Al4 Gd1 63.01(2) 4_565 3
Al4 Al4 Gd1 63.05(2) 8 3
Al1 Al4 Gd1 126.75(4) 14_556 3
Al1 Al4 Gd1 68.50(2) . 3
Mo3 Al4 Gd1 167.32(4) 14_556 3
Al6 Al4 Gd1 167.32(4) 14_556 3
Al6 Al4 Gd1 66.350(19) . 3
Mo1 Al4 Gd1 75.03(2) 3 18_556
Al1 Al4 Gd1 63.01(2) 17_566 18_556
Al1 Al4 Gd1 122.19(4) 4_565 18_556
Al4 Al4 Gd1 63.05(2) 8 18_556
Al1 Al4 Gd1 68.50(2) 14_556 18_556
Al1 Al4 Gd1 126.75(4) . 18_556
Mo3 Al4 Gd1 66.350(19) 14_556 18_556
Al6 Al4 Gd1 66.350(19) 14_556 18_556
Al6 Al4 Gd1 167.32(4) . 18_556
Gd1 Al4 Gd1 126.00(4) 3 18_556
Al3 Al5 Al3 66.25(5) 5_554 18_556
Al3 Al5 Al6 109.55(3) 5_554 .
Al3 Al5 Al6 130.70(3) 18_556 .
Al3 Al5 Mo3 130.70(3) 5_554 10_665
Al3 Al5 Mo3 109.55(3) 18_556 10_665
Al6 Al5 Mo3 107.80(5) . 10_665
Al3 Al5 Al6 130.70(3) 5_554 10_665
Al3 Al5 Al6 109.55(3) 18_556 10_665
Al6 Al5 Al6 107.80(5) . 10_665
Mo3 Al5 Al6 0.00(3) 10_665 10_665
Al3 Al5 Al5 118.05(3) 5_554 3_665
Al3 Al5 Al5 168.59(3) 18_556 3_665
Al6 Al5 Al5 59.32(2) . 3_665
Mo3 Al5 Al5 59.32(2) 10_665 3_665
Al6 Al5 Al5 59.32(2) 10_665 3_665
Al3 Al5 Al5 168.59(3) 5_554 4_565
Al3 Al5 Al5 118.05(3) 18_556 4_565
Al6 Al5 Al5 59.32(2) . 4_565
Mo3 Al5 Al5 59.32(2) 10_665 4_565
Al6 Al5 Al5 59.32(2) 10_665 4_565
Al5 Al5 Al5 60.0 3_665 4_565
Al3 Al5 Gd1 67.56(3) 5_554 16
Al3 Al5 Gd1 104.81(4) 18_556 16
Al6 Al5 Gd1 119.00(2) . 16
Mo3 Al5 Gd1 66.659(11) 10_665 16
Al6 Al5 Gd1 66.659(11) 10_665 16
Al5 Al5 Gd1 69.37(2) 3_665 16
Al5 Al5 Gd1 118.86(2) 4_565 16
Al3 Al5 Gd1 104.81(4) 5_554 3
Al3 Al5 Gd1 67.56(3) 18_556 3
Al6 Al5 Gd1 66.658(11) . 3
Mo3 Al5 Gd1 119.00(2) 10_665 3
Al6 Al5 Gd1 119.00(2) 10_665 3
Al5 Al5 Gd1 118.86(2) 3_665 3
Al5 Al5 Gd1 69.37(2) 4_565 3
Gd1 Al5 Gd1 171.37(5) 16 3
Al3 Al5 Gd1 63.14(2) 5_554 4_665
Al3 Al5 Gd1 128.48(4) 18_556 4_665
Al6 Al5 Gd1 62.458(9) . 4_665
Mo3 Al5 Gd1 110.03(2) 10_665 4_665
Al6 Al5 Gd1 110.03(2) 10_665 4_665
Al5 Al5 Gd1 58.76(2) 3_665 4_665
Al5 Al5 Gd1 110.03(2) 4_565 4_665
Gd1 Al5 Gd1 63.911(8) 16 4_665
Gd1 Al5 Gd1 117.070(9) 3 4_665
Al3 Al5 Gd1 128.48(4) 5_554 15_565
Al3 Al5 Gd1 63.14(2) 18_556 15_565
Al6 Al5 Gd1 110.03(2) . 15_565
Mo3 Al5 Gd1 62.458(10) 10_665 15_565
Al6 Al5 Gd1 62.458(10) 10_665 15_565
Al5 Al5 Gd1 110.03(2) 3_665 15_565
Al5 Al5 Gd1 58.76(2) 4_565 15_565
Gd1 Al5 Gd1 117.070(9) 16 15_565
Gd1 Al5 Gd1 63.911(9) 3 15_565
Gd1 Al5 Gd1 168.32(4) 4_665 15_565
Al1 Al6 Al1 114.30(3) 4_565 3_665
Al1 Al6 Al1 114.30(3) 4_565 .
Al1 Al6 Al1 114.30(3) 3_665 .
Al1 Al6 Al5 68.42(3) 4_565 4_565
Al1 Al6 Al5 113.46(3) 3_665 4_565
Al1 Al6 Al5 123.95(4) . 4_565
Al1 Al6 Al5 113.46(3) 4_565 .
Al1 Al6 Al5 123.95(4) 3_665 .
Al1 Al6 Al5 68.42(3) . .
Al5 Al6 Al5 61.36(4) 4_565 .
Al1 Al6 Al5 123.95(4) 4_565 3_665
Al1 Al6 Al5 68.42(3) 3_665 3_665
Al1 Al6 Al5 113.46(3) . 3_665
Al5 Al6 Al5 61.36(4) 4_565 3_665
Al5 Al6 Al5 61.36(4) . 3_665
Al1 Al6 Al4 61.03(3) 4_565 4_565
Al1 Al6 Al4 59.55(4) 3_665 4_565
Al1 Al6 Al4 115.35(5) . 4_565
Al5 Al6 Al4 113.16(3) 4_565 4_565
Al5 Al6 Al4 174.04(3) . 4_565
Al5 Al6 Al4 119.00(3) 3_665 4_565
Al1 Al6 Al4 59.55(4) 4_565 .
Al1 Al6 Al4 115.35(5) 3_665 .
Al1 Al6 Al4 61.03(3) . .
Al5 Al6 Al4 119.00(3) 4_565 .
Al5 Al6 Al4 113.16(3) . .
Al5 Al6 Al4 174.04(3) 3_665 .
Al4 Al6 Al4 66.71(4) 4_565 .
Al1 Al6 Al4 115.35(5) 4_565 3_665
Al1 Al6 Al4 61.03(3) 3_665 3_665
Al1 Al6 Al4 59.55(4) . 3_665
Al5 Al6 Al4 174.04(3) 4_565 3_665
Al5 Al6 Al4 119.00(3) . 3_665
Al5 Al6 Al4 113.16(3) 3_665 3_665
Al4 Al6 Al4 66.71(4) 4_565 3_665
Al4 Al6 Al4 66.71(4) . 3_665
Al1 Al6 Gd1 61.167(18) 4_565 3
Al1 Al6 Gd1 174.86(5) 3_665 3
Al1 Al6 Gd1 67.277(19) . 3
Al5 Al6 Gd1 67.833(17) 4_565 3
Al5 Al6 Gd1 61.170(16) . 3
Al5 Al6 Gd1 115.83(5) 3_665 3
Al4 Al6 Gd1 115.31(3) 4_565 3
Al4 Al6 Gd1 60.69(2) . 3
Al4 Al6 Gd1 117.87(3) 3_665 3
Al1 Al6 Gd1 67.277(19) 4_565 1_565
Al1 Al6 Gd1 61.167(18) 3_665 1_565
Al1 Al6 Gd1 174.86(5) . 1_565
Al5 Al6 Gd1 61.170(16) 4_565 1_565
Al5 Al6 Gd1 115.83(5) . 1_565
Al5 Al6 Gd1 67.833(17) 3_665 1_565
Al4 Al6 Gd1 60.69(2) 4_565 1_565
Al4 Al6 Gd1 117.87(3) . 1_565
Al4 Al6 Gd1 115.31(3) 3_665 1_565
Gd1 Al6 Gd1 117.009(14) 3 1_565
Al1 Al6 Gd1 174.86(5) 4_565 4_665
Al1 Al6 Gd1 67.277(19) 3_665 4_665
Al1 Al6 Gd1 61.167(18) . 4_665
Al5 Al6 Gd1 115.83(5) 4_565 4_665
Al5 Al6 Gd1 67.833(17) . 4_665
Al5 Al6 Gd1 61.170(16) 3_665 4_665
Al4 Al6 Gd1 117.87(3) 4_565 4_665
Al4 Al6 Gd1 115.31(3) . 4_665
Al4 Al6 Gd1 60.69(2) 3_665 4_665
Gd1 Al6 Gd1 117.009(14) 3 4_665
Gd1 Al6 Gd1 117.009(14) 1_565 4_665
Mo1 Al7 Mo1 173.41(8) 3_655 4_655
Mo1 Al7 Al7 56.71(4) 3_655 4_765
Mo1 Al7 Al7 116.71(4) 4_655 4_765
Mo1 Al7 Al7 116.71(4) 3_655 3_645
Mo1 Al7 Al7 56.71(4) 4_655 3_645
Al7 Al7 Al7 60.0 4_765 3_645
Mo1 Al7 Al1 124.77(5) 3_655 3_655
Mo1 Al7 Al1 60.30(2) 4_655 3_655
Al7 Al7 Al1 146.17(3) 4_765 3_655
Al7 Al7 Al1 107.28(3) 3_645 3_655
Mo1 Al7 Al1 60.30(2) 3_655 8_655
Mo1 Al7 Al1 124.77(5) 4_655 8_655
Al7 Al7 Al1 107.28(3) 4_765 8_655
Al7 Al7 Al1 146.17(3) 3_645 8_655
Al1 Al7 Al1 98.75(6) 3_655 8_655
Mo1 Al7 Al1 124.77(5) 3_655 18_656
Mo1 Al7 Al1 60.30(2) 4_655 18_656
Al7 Al7 Al1 146.17(3) 4_765 18_656
Al7 Al7 Al1 107.28(3) 3_645 18_656
Al1 Al7 Al1 65.32(5) 3_655 18_656
Al1 Al7 Al1 64.51(5) 8_655 18_656
Mo1 Al7 Al1 60.30(2) 3_655 23_655
Mo1 Al7 Al1 124.77(5) 4_655 23_655
Al7 Al7 Al1 107.28(3) 4_765 23_655
Al7 Al7 Al1 146.17(3) 3_645 23_655
Al1 Al7 Al1 64.51(5) 3_655 23_655
Al1 Al7 Al1 65.32(5) 8_655 23_655
Al1 Al7 Al1 98.75(6) 18_656 23_655
Mo1 Al7 Al2 57.95(2) 3_655 18_656
Mo1 Al7 Al2 120.09(3) 4_655 18_656
Al7 Al7 Al2 61.43(3) 4_765 18_656
Al7 Al7 Al2 92.21(4) 3_645 18_656
Al1 Al7 Al2 151.92(6) 3_655 18_656
Al1 Al7 Al2 56.51(3) 8_655 18_656
Al1 Al7 Al2 89.99(3) 18_656 18_656
Al1 Al7 Al2 109.31(4) 23_655 18_656
Mo1 Al7 Al2 120.09(3) 3_655 4_655
Mo1 Al7 Al2 57.95(2) 4_655 4_655
Al7 Al7 Al2 92.21(4) 4_765 4_655
Al7 Al7 Al2 61.43(3) 3_645 4_655
Al1 Al7 Al2 56.51(3) 3_655 4_655
Al1 Al7 Al2 151.92(6) 8_655 4_655
Al1 Al7 Al2 109.31(4) 18_656 4_655
Al1 Al7 Al2 89.99(3) 23_655 4_655
Al2 Al7 Al2 150.59(7) 18_656 4_655
Mo1 Al7 Al2 120.09(3) 3_655 17_656
Mo1 Al7 Al2 57.95(2) 4_655 17_656
Al7 Al7 Al2 92.21(4) 4_765 17_656
Al7 Al7 Al2 61.43(3) 3_645 17_656
Al1 Al7 Al2 109.31(4) 3_655 17_656
Al1 Al7 Al2 89.99(3) 8_655 17_656
Al1 Al7 Al2 56.51(3) 18_656 17_656
Al1 Al7 Al2 151.92(6) 23_655 17_656
Al2 Al7 Al2 62.24(5) 18_656 17_656
Al2 Al7 Al2 109.69(4) 4_655 17_656
Mo1 Al7 Al2 57.95(2) 3_655 3_655
Mo1 Al7 Al2 120.09(3) 4_655 3_655
Al7 Al7 Al2 61.43(3) 4_765 3_655
Al7 Al7 Al2 92.21(4) 3_645 3_655
Al1 Al7 Al2 89.99(3) 3_655 3_655
Al1 Al7 Al2 109.31(4) 8_655 3_655
Al1 Al7 Al2 151.92(6) 18_656 3_655
Al1 Al7 Al2 56.51(3) 23_655 3_655
Al2 Al7 Al2 109.69(4) 18_656 3_655
Al2 Al7 Al2 62.24(5) 4_655 3_655
Al2 Al7 Al2 150.59(7) 17_656 3_655
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Gd1 Al1 3.0700(9) 23_655
Gd1 Al1 3.0700(9) 3_655
Gd1 Al4 3.0921(6) 9
Gd1 Al4 3.0921(6) 4
Gd1 Al5 3.0994(3) 15
Gd1 Al5 3.0994(3) 4
Gd1 Mo3 3.2484(4) 22
Gd1 Al6 3.2484(4) 22
Gd1 Mo3 3.2484(4) 1_545
Gd1 Al6 3.2484(4) 1_545
Gd1 Al3 3.2588(12) 2_654
Gd1 Al3 3.2608(12) 14_556
Mo1 Al7 2.5670(4) 3_545
Mo1 Al7 2.5670(4) 4_665
Mo1 Al4 2.6905(13) 9
Mo1 Al4 2.6905(13) 4
Mo1 Al2 2.6917(12) .
Mo1 Al2 2.6917(12) 14_556
Mo1 Al1 2.7200(9) 9
Mo1 Al1 2.7200(9) 4
Mo1 Al1 2.7199(9) 17_556
Mo1 Al1 2.7200(9) 22
Mo1 Gd1 3.5359(4) 14_556
Mo2 Al2 2.6903(12) 15
Mo2 Al2 2.6903(12) 3
Mo2 Al2 2.6903(12) 13
Mo2 Al2 2.6903(12) .
Mo2 Al2 2.6903(12) 16
Mo2 Al2 2.6903(12) 4
Mo2 Al3 2.8462(12) 17_556
Mo2 Al3 2.8462(12) 5_554
Mo2 Al3 2.8462(12) 18_556
Mo2 Al3 2.8462(12) 14_556
Mo2 Al3 2.8462(12) 2_554
Mo2 Al3 2.8462(12) 6_554
Al1 Al6 2.7186(10) .
Al1 Mo1 2.7200(9) 3
Al1 Al2 2.7362(11) 3
Al1 Al4 2.7575(13) 3_665
Al1 Al4 2.8197(13) .
Al1 Al7 2.8291(14) 4_665
Al1 Al3 2.8981(14) 5_554
Al1 Gd1 3.0700(9) 4_665
Al1 Gd1 3.3347(9) 3
Al2 Al1 2.7362(11) 22
Al2 Al1 2.7362(11) 4
Al2 Al3 2.7750(17) 14_556
Al2 Al3 2.8691(12) 6_554
Al2 Al3 2.8691(12) 5_554
Al2 Al7 2.9465(12) 4_665
Al2 Al7 2.9465(12) 3_545
Al3 Al5 2.7403(12) 6
Al3 Al5 2.7403(12) 17_556
Al3 Al2 2.7750(17) 14_556
Al3 Mo2 2.8462(12) 2
Al3 Al2 2.8691(12) 5
Al3 Al2 2.8691(12) 6
Al3 Al1 2.8981(14) 6
Al3 Al1 2.8981(14) 20_556
Al3 Al3 2.9950(15) 15_556
Al3 Al3 2.9950(15) 16_556
Al3 Gd1 3.2588(12) 2_655
Al3 Gd1 3.2608(12) 14_556
Al4 Mo1 2.6905(13) 3
Al4 Al1 2.7575(13) 17_566
Al4 Al1 2.7575(13) 4_565
Al4 Al4 2.803(3) 8
Al4 Al1 2.8197(13) 14_556
Al4 Mo3 2.8308(13) 14_556
Al4 Al6 2.8308(13) 14_556
Al4 Al6 2.8308(13) .
Al4 Gd1 3.0921(6) 3
Al4 Gd1 3.0921(6) 18_556
Al5 Al3 2.7403(12) 5_554
Al5 Al3 2.7403(12) 18_556
Al5 Al6 2.7945(13) .
Al5 Mo3 2.7945(13) 10_665
Al5 Al6 2.7945(13) 10_665
Al5 Al5 2.852(2) 3_665
Al5 Al5 2.852(2) 4_565
Al5 Gd1 3.0994(3) 16
Al5 Gd1 3.0994(3) 3
Al5 Gd1 3.3928(3) 4_665
Al5 Gd1 3.3928(3) 15_565
Al6 Al1 2.7186(10) 4_565
Al6 Al1 2.7186(10) 3_665
Al6 Al5 2.7945(13) 4_565
Al6 Al5 2.7945(13) 3_665
Al6 Al4 2.8308(13) 4_565
Al6 Al4 2.8309(13) 3_665
Al6 Gd1 3.2484(4) 3
Al6 Gd1 3.2484(4) 1_565
Al6 Gd1 3.2484(4) 4_665
Al7 Mo1 2.5670(4) 3_655
Al7 Mo1 2.5670(4) 4_655
Al7 Al7 2.818(3) 4_765
Al7 Al7 2.818(3) 3_645
Al7 Al1 2.8291(14) 3_655
Al7 Al1 2.8291(14) 8_655
Al7 Al1 2.8291(14) 18_656
Al7 Al1 2.8291(14) 23_655
Al7 Al2 2.9466(12) 18_656
Al7 Al2 2.9466(12) 4_655
Al7 Al2 2.9466(12) 17_656
Al7 Al2 2.9466(12) 3_655
